Talc is employed in low fire bodies to raise their thermal expansion (to put the squeeze on glazes to prevent crazing). These dilatometer curves make it very clear just how effective that strategy is! The talc body was fired at cone 04, the stoneware at cone 6. The former is porous and completely non-vitreous, the latter is semi vitreous. This demonstrates something else interesting: The impracticality of calculating the thermal expansion of clay bodies based on their oxide chemistry. Talc sources MgO and low fire bodies containing it would calculate to a low thermal expansion. But the opposite happens. Why? Because these bodies are composed of mineral particles loosely sintered together. A few melt somewhat, some change their mineral form, most remain unchanged. The body's COE is the additive sum of the proportionate populations of all the particles. Good luck calculating that!
Co-efficient of Thermal Expansion
Ceramics are brittle and many types will crack if subjected to sudden heating or cooling. Some do not. Why? Differences in their co-efficients of thermal expansion.
Shivering is a ceramic glaze defect that results in tiny flakes of glaze peeling off edges of ceramic ware. It happens because the thermal expansion of the body is too much higher than the glaze.
Calculated Thermal Expansion
The thermal expansion of a glaze can be predicted (relatively) and adjusted using simple glaze chemistry. Body expansion cannot be calculated.
Low Fire White Talc Casting Body Recipe
The classic white ball clay talc casting and modelling recipe has been used for many years. It is a dream to use as long as you are aware of the problems and risks.
G1916Q - Low Fire Highly-Expansion-Adjustable Transparent
An expansion-adjustable cone 04-02 transparent glaze made using three common Ferro frits (low and high expansion), it produces an easy-to-use slurry.
Sign up at the home page.